Macromolecules - Rensselaer Polytechnic grossr/_doc/publication/Macromolecules 1993 آ ...
Embed Size (px)
Transcript of Macromolecules - Rensselaer Polytechnic grossr/_doc/publication/Macromolecules 1993 آ ...
Macromolecules Volume 26, Number 23 November 8, 1993
0 Copyright 1993 by the American Chemical Society
Syndiospecific Ring-Opening Polymerization of P-Butyrolactone To Form Predominantly Syndiotactic Poly(P-hydroxybutyrate) Using Tin(1V) Catalysts
John E. Kemnitzer? Stephen P. McCarthy? and Richard A. Gross**+ Departments of Chemistry and Plastics Engineering, University of Massachusetts, Lowell, Lowell, Massachusetts 01854
Received May 13, 1993; Reuised Manuscript Received August 16, 199P
ABSTRACT: In a previous report, we have documented the ability of tri-n-butyltin methoxide (Sn(n- Bu)aOCHs) to catalyze the ring-opening polymerization of racemic fl-butyrolactone ((h)-BL) to form poly- (fl-hydroxybutyrate) (PHB) with a preference for syndiotactic (syn) placement. In this report, bis(tri-n- butyltin) oxide ((n-BusSn)zO), bis(tripheny1tin) oxide (PhsSn)zO), and di-n-butyltin dimethoxide (Sn(n- Bu)*(OCH&) were all shown to catalyze the syndiospecific polymerization of (h)-BL. Of these catalysts, the Sn(n-Bu)z(OCH& system showed dramatically decreased polymerization times for correspondingly high monomer conversion. This catalyst system was used to form syn-PHB with an M, and syn diad fraction of 8.4 X l@ and 0.62, respectively. Analysis of the stereochemical sequence distributions a t various polymerization temperatures for all of the Sn(1V) catalysts investigated showed an (E, - Ei) of ca. -2 kcallmol for syndiotactic versus isotactic diad formation. Therefore, the syndiospecificity exhibited little dependence on the catalyst structure over a limited, but significantly broad range of Sn(1V) organometallic systems. The triad stereosequence distributions of syn-PHB samples agrees very well with the Bernoulli model of chain end stereocontrol. Furthermore, the degree of Sn(1V)-catalyst syndiospecificity increased a t correspondingly lower polymerization temperatures. Polymerizations carried out a t -15 and +90 OC with the Sn(n-Bu)Z- (OCH& catalyst system gave syn-PHB with syn diad fractions of 0.72 and 0.54, respectively. The polymers formed from (R)-BL (>98% ee) all showed significant (-13%) degrees of configurational inversion a t the stereogenic center, with little dependence on the catalyst used or the polymerization temperature. This result indicates that while the preferred mode of ring opening is primarily acyl cleavage (bond breaking between the carbonyl carbon and oxygen of the lactone), a mechanism for stereocenter inversion is operative.
Introduction Classical synthetic methods can be used to obtain
structures which mimic those found in nature. An ex- cellent example of such work is that which has been carried out for the preparation of the poly(@-hydroxybutyrate) (PHB) from butyrolactone (BL) using various organo- metallic species to catalyze the ring-opening polymeri- ~a t ion . l -~ The corresponding natural polymer (R)-PHB is a member of a family of poly(@-hydroxyalkanoates) (PHAs) that are formed by a wide variety of bacteria.'* An important consideration for the purposes of this paper is that the natural polymer has t o date been found exclusively in the enantiomerically pure form where the stereocenters are in the (R) configuration. Clearly, an important ad- vantage associated with the ring-opening route to PHB
* To whom correspondence should be addressed. f Department of Chemistry.
e Abstract published in Advance ACS Abstracts, October 1,1993. Department of Plastics Engineering.
and other PHAs is the possibility of preparing these polymers in a variety of stereochemical forms having tailored physical and biological characteristics.
There has been increased interest in the use of PHB synthetic analogues as biodegradable polymers. In ad- dition, PHB synthetic analogs have been viewed as interesting model systems to investigate effects of ster- eochemical and morphological parameters on the biodeg- radation kinetics. In our laboratory, we have investigated the relative enzymatic degradability of random PHB stereocopolymers containing various (R)-hydroxybutyrate ((R)-HB) contents (4-100% ).ll This study was performed using a depolymerase isolated from Penicillium funicu- losum, and the initial surface degradation rate was measured by monitoring pH change. It was found that the preference for (R)-HB repeat units appears to dominate over crystalline morphology effects for the compositional range 81-100 % (R)-HB. However, dramatically larger initial surface degradation rate values observed for 67 and 77% (R)-HB contents suggested that a critical degree of
0 1993 American Chemical Society
6144 Kemnitzer et al. Macromolecules, Vol. 26, No. 23, 1993
pounds, has recently been described by Kricheldorf and ~ o - w o r k e r s . 6 ~ ~ ~ ~ ~ They have demonstrated that tributyltin methoxide is very active in the polymerization of e-cap- rolactone, (L,L)-lactide, 0-propiolactone, and BL.5v23.24 Mechanistic studies carried out by these workers indicate that the lactone polymerizations proceed by a coordina- tion-insertion mechanism where chain growth involves cleavage of the acyl-oxygen lactone bond and yields polyester chains with a methyl ester end g r o ~ p . ~ ~ ~ ~ ~ Recently, our laboratory has reported that (*)-BL po- lymerization by the Sn(1V) catalyst Sn(n-Bu)3OCH3 resulted in the preparation of syn-PHB with racemic (r) diad fractions as high as 0.70.15 It was also found by lH NMR end group analysis that the polymers formed did not have predominantly methyl ester end groups. In fact, the ratio of carboxylic acid to methyl ester end groups ranged from 2.5 to 3.1.15 The syn-PHB samples that were prepared were found to be crystalline and had a crystalline structure which was different from that of bacterial PHB.I5
In this paper, the syndiospecificity of the Sn(1V) catalysts bis(tri-n-butyltin) oxide ((n-BusSn)ZO), bis- (triphenyltin) oxide ((PhsSn)zO), and di-n-butyltin dimethoxide (Sn(n-Bu)z(OCHs)z) for the formation of syn- PHB from (*)-BL was investigated. The temperature effect on syndiospecificity was used to determine the activation energy (At3 = E, - Ei) for syndiotactic versus isotactic diad placement. Polymerization of enantiomer- ically pure BL and determination of the corresponding polymer stereochemistry were used to determine the preferred mode of ring opening (acyl vs alkyl cleavage) as well as whether mechanisms for stereochemical inversion are operative.
disruption of the crystalline order occurred at these stereochemical compositions accelerating the observed degradation kinetics. Furthermore, it was shown that 50% (R)-atactic PHB (Mn = 50000) was a poor substrate for the enzyme after rapid initial surface degradation of (R)- HB-rich polymer chain segments a t the film surface. In contrast, 50% (R)-syndiotactic PHB (Mn = 9200, syn diad fraction of 0.66) was found to be degradable by the depolymerase of P. funicolusum both in short- and long- term studies. Kumagai and Doi have reported on the enzymatic degradability of (R)-PHB (natural origin) blended with (R,S)-atactic PHB.12 The degradation measurements were made by exposure of these blends to the extracellular PHB depolymerase isolated from Al- caligenes faecalis T1.12 It was shown that the rate of enzyme-mediated blend biodegradation (as measured by weight loss) increased with increasing content of the (8,s)- atactic PHB such that the highest rate was observed at a 50 wt 7% blend. Furthermore, it was reported that the blend component @,SI-atactic PHB was degraded by the A . faecalis depolymerase to form 3-hydroxybutyric acid and oligomers, although the rate of biodegradation was relatively slower than that measured for (R)-PHB.13 Pearce et al. have studied blends of bacterial PHB and predominantly isotactic and atactic 50 5% (R)-PHB.14 Blends of predominantly isotactic 50% (R)-PHB and bacterial PHB showed a single melting point which decreased with increasing 50 % (R)-isotactic PHB blend content. In addition, the melting point of these blends was between that of its component materials. Therefore, it was concluded by these workers that the two components are cocrystallizing and that the inclusion is essentially complete. In contrast, synthetic atactic PHB was found to be incompatible with the bacterial PHB.14
The first preparation of predominantly syn-PHB was reported as part of a study directed at the measurement of initial surface degradation kinetics of PHB stereoco- polymers.ll That study, carried out in our laboratory, was summarized above. Further work by our research group documented the preparation of predominantly syn- PHB from (d=)-BL using tri-n-butyltin methoxide as ~atalyst . '~ Interestingly, to our knowledge, these exper- imental results provided the first example of a syndiospe- cific ring-opening polymerization. More recently, Hocking and MarchessaultlG observed that polymerization of (A)- BL catalyzed by methylaluminoxane gave a product fraction that was syn-PHB. Unfortunately, using this approach, the maximum conversion of monomer to syn- PHB was only 2 96. In addition, typical M , and M,, values of the syn-PHB fraction were ca. 3000 and 600, respectively, and racemic diad fractions up to 0.68 were measured. The major products of (*)-BL polymerization catalyzed by methylaluminoxane, as well as other aluminum-based catalyst systems derived from trialkylaluminumlwater, are relatively higher molecular weight predominantly isotactic PHB.lGZ2 I t is interesting to note that the observation by Hocking and Marchessault16 of drastically different active site catalyst mechanisms present in methylaluminoxane polymerizations resulting in